Porphyrin based push‒pull conjugates as donors for solution-processed bulk heterojunction solar cells: a case of metal-dependent power conversion efficiency
Mishra, Ruchika; Regar, Ramprasad; Singhal, Rahul; Panini, Piyush; Sharma, Ganesh D.; Sankar, Jeyaraman; Journal of Materials Chemistry A 5 (2017) 15529–; doi:10.1039/C7TA05338J

data_7236605
_publ_section_title
;
 Porphyrin based push--pull conjugates as donors for solution-processed
 bulk heterojunction solar cells: a case of metal-dependent power
 conversion efficiency
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry A'
_journal_page_first              15529
_journal_paper_doi               10.1039/C7TA05338J
_journal_volume                  5
_journal_year                    2017
_chemical_formula_sum            'C84 H70 N8 Ni O4'
_chemical_formula_weight         1314.19
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2016/6
_audit_update_record
;
2017-02-06 deposited with the CCDC.
2017-07-12 downloaded from the CCDC.
;
_cell_angle_alpha                91.948(6)
_cell_angle_beta                 98.062(6)
_cell_angle_gamma                114.160(5)
_cell_formula_units_Z            4
_cell_length_a                   17.631(2)
_cell_length_b                   18.379(3)
_cell_length_c                   24.555(3)
_cell_measurement_temperature    110(2)
_cell_volume                     7151.2(17)
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      110(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.3479
_diffrn_reflns_av_unetI/netI     0.2892
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            169701
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_min         2.231
_exptl_absorpt_coefficient_mu    0.328
_exptl_crystal_density_diffrn    1.221
_exptl_crystal_F_000             2760
_refine_diff_density_max         0.994
_refine_diff_density_min         -0.795
_refine_diff_density_rms         0.108
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1446
_refine_ls_number_reflns         25154
_refine_ls_number_restraints     540
_refine_ls_restrained_S_all      1.062
_refine_ls_R_factor_all          0.3073
_refine_ls_R_factor_gt           0.1506
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1691P)^2^+16.4087P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3299
_refine_ls_wR_factor_ref         0.3937
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9901
_reflns_number_total             25154
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7ta05338j2.cif
_cod_data_source_block           shelx
_cod_database_code               7236605
_shelx_shelxl_version_number     2016/6
_shelx_res_checksum              16160
_shelx_fab_checksum              18358